multistep lithiation of tin sulfide: an investigation ... ... multistep lithiation of tin...
Post on 16-Jul-2020
Embed Size (px)
Multistep Lithiation of Tin Sulfide: An Investigation Using in Situ Electron Microscopy Sooyeon Hwang,† Zhenpeng Yao,‡ Lei Zhang,§ Maosen Fu,∥,† Kai He,‡ Liqiang Mai,§
Chris Wolverton,‡ and Dong Su*,†
†Center for Functional Nanomaterials, Brookhaven National Laboratory, Upton, New York 11973, United States ‡Department of Materials Science and Engineering, Northwestern University, Evanston, Illinois 60208, United States §State Key Laboratory of Advanced Technology for Materials Synthesis and Processing, Wuhan University of Technology, Wuhan 430070, P. R. China ∥Shanxi Materials Analysis and Research Center, School of Materials Science and Engineering, Northwestern Polytechnical University, Xi’an 710000, P. R. China
*S Supporting Information
ABSTRACT: Two-dimensional (2D) metal sulfides have been widely explored as promising electrodes for lithium- ion batteries since their two-dimensional layered structure allows lithium ions to intercalate between layers. For tin disulfide, the lithiation process proceeds via a sequence of three different types of reactions: intercalation, conversion, and alloying, but the full scenario of reaction dynamics remains nebulous. Here, we investigate the dynamical pro- cess of the multistep reactions using in situ electron micros- copy and discover the formation of an intermediate rock- salt phase with the disordering of Li and Sn cations after initial 2D intercalation. The disordered cations occupy all the octahedral sites and block the channels for intercalation, which alter the reaction pathways during further lithiation. Our first-principles calculations of the nonequilibrium lithiation of SnS2 corroborate the energetic preference of the disordered rock-salt structure over known layered polymorphs. The in situ observations and calculations suggest a two-phase reaction nature for intercalation, disordering, and following conversion reactions. In addition, in situ delithiation observation confirms that the alloying reaction is reversible, while the conversion reaction is not, which is consistent with the ex situ analysis. This work reveals the full lithiation characteristic of SnS2 and sheds light on the understanding of complex multistep reactions in 2D materials.
KEYWORDS: lithium-ion batteries, in situ transmission electron microscopy, tin disulfide, multistep lithiation, density functional theory
Current widespread usage of lithium-ion batteries (LIBs)in a number of electronic devices has been realized byusing intercalation-type of electrode materials, such as carbonaceous materials and lithium transition-metal oxides.1,2
As lithium ions can be inserted into and extracted from empty spaces inside electrode materials, the original structures of host compounds are well maintained during operation, which improves reversibility and long-term stability. Despite their success in market, these kinds of materials have intrinsic limitations on energy density because of the limited number of vacant sites inside host compounds. Conversion-type nanosized mate- rials (metal oxides, sulfides, fluorides, etc.)3−8 and alloying-type materials (Si, Sb, Ge, Sn, etc.)9,10 can be attractive alternatives which offer much higher energy density for LIBs. However, these types of materials also have problematic issues, for example, volume expansion, mechanical integrity, reversibility, and long- term stability. The mechanism by which electrode materials store Li ions governs the characteristics of battery cells; therefore,
thorough understanding of the lithiation process is of importance for improving the figures-of-merits of electrode materials. Some metal chalcogenides which adopt a two-dimensional
(2D) layered structure have exhibited intriguing lithium inser- tion reactions. Since adjacent metal sulfur layers are bonded by the relatively weak van der Waals force,11,12 Li-ions can be inter- calated between these adjacent metal−sulfur layers. This charac- teristic has made metal chalcogenides draw an intensive amount of attention as electrode materials in late 1970s.13,14 Despite the similar 2D structure across many chalcogenides,11,13,15,16 differ- ent metal sulfides may have distinct lithiation reaction mecha- nisms. In case of MoS2, the intercalation of Li ions is accom- panied by a Mo coordination change from trigonal prismatic to
Received: January 29, 2018 Accepted: April 3, 2018 Published: April 3, 2018
le www.acsnano.orgCite This: ACS Nano 2018, 12, 3638−3645
© 2018 American Chemical Society 3638 DOI: 10.1021/acsnano.8b00758 ACS Nano 2018, 12, 3638−3645
www.acsnano.org http://pubs.acs.org/action/showCitFormats?doi=10.1021/acsnano.8b00758 http://dx.doi.org/10.1021/acsnano.8b00758
octahedral,17 followed by a conversion process from LixMoS2 to Li2S and Mo.
18 For copper sulfides (CuS, Cu2S), after the intercalation reaction, an extrusion (displacement) reaction takes place rather than the conversion reaction.19−21 Among these 2D layered chalcogenides, SnS2 has an interesting and complicated reaction nature with lithium, which featured with consequently connected three different types of reactions: inter- calation, conversion, and alloying:22,23
+ + →+ −SnS Li e Li SnSx2 2 (1)
+ − + − → ++ −x xLi SnS (4 )Li (4 )e Sn 2Li Sx 2 2 (2)
+ ↔Sn 4.4Li Li Sn4.4 (3)
It is believed that the conversion reaction is not reversible which largely instigates a low Coulombic efficiency during the first cycle.24−26 Thus, only 645 mAh/g originated from alloying reaction is reversible, while the theoretical capacity for whole reaction is up to 1231 mAh/g. As electrochemical performance is highly dependent on how these reactions proceed, for example, the reaction pathways, intermediate phases involving this com- plicated reaction process,22,23,27,28 real-time investigation is necessary to improve figure-of-merits of electrode materials. A couple of studies performed in situ electron microscopy work of SnS2: Gao et al.
27 studied the intercalation and deinter- calation processes, and Yin et al.28 reported formation of self- assembled composite framework after the first discharge process. However, up to now, the microscopic investigation on the whole different types of lithiation reactions still lacks for SnS2, and insights regarding a full scenario of reaction dynamics remain elusive. Herein, we perform a mechanistic study on the lithiation and
delithiation processes of tin disulfide using in situ transmission electron microscopy (TEM) in combination with first-principles calculations. Our in situ selected area electron diffraction (SAED) and scanning TEM (STEM) results elucidate four sequential reaction steps during the lithiation of SnS2. A disordering transition with the formation of rock-salt phase is discovered after initial intercalation. The rearrangement of cations happens with Li and Sn equally occupying the octahedral sites and completely changes the structure of the layered compound, making the Li-intercalation impossible. After the disordering transition, further lithiation will prompt a conversion reaction with the collapse of crystal lattice. We note that the electron beam may induce phase transition in the electrode materials for batteries.29 To avoid that issue, we here performed the in situ STEM imaging at a dose rate around 0.3 pA/cm2. In addition, DFT calculations are conducted to explore a variety of possible lithiation reaction pathways of SnS2 and identify the ground- state reaction path, which validates the experimental observa- tions. Precise real-time analysis performed here reveals full reaction natures of tin sulfides which cannot be acquired by post-mortem studies.
RESULTS AND DISCUSSION Figure 1a−c shows scanning electron microscopy (SEM), high angle annular dark-field (HAADF)-scanning transmission elec- tron microscopy (STEM), and high-resolution transmission electron microscopy (HRTEM) images of flower-like tin disulfide (SnS2) samples studied in this work. Micron-sized flower samples are composed of pile-up of thin sheets. Figure S1a,c presents an X-ray diffraction pattern and HRTEM image along the  zone axis of SnS2, indicating a 2H structure of space group P3m̅1.
STEM-electron energy loss spectroscopy (EELS) elemental maps in Figure S1b demonstrate the uniform distribution of Sn and S in SnS2. The electrochemical activity of SnS2 was examined in a coin cell, as shown in Figure S2. SAED patterns at pristine, discharged (0.01 V), and charged (3 V) states (Figure 1d−f, respectively) demonstrate that lithiation of SnS2 results in formations of Li−Sn alloy phase, Li7Sn2, and removal of lithium ions leads to dealloying of Li−Sn instead of structural recovery of SnS2. This is consistent with the previous reports.
Real-time structural evolutions of SnS2 during the lithium insertion were examined with both in situ electron diffraction and in situ imaging. We took advantage of a dry-format electrochemical cell setup.31−34 We used Li/Li2O on STM tip as the counter electrode/solid electrolyte and SnS2 on lacey carbon Cu TEM grid as the active electrode for in situ exper- iments. Figure 2a presents radial intensity profiles as a function of reaction time produced from real-time SAEDs. The details of the data processing can be found in Figure S3. Raw video and SAED patterns are presented in Movie S1 and Figure S4, respectively. When lithium ions are introduced to SnS2, the phase transitions can be determined by the modifications in radial intensity profiles (peak shift, disappearance or appearance of peaks). The radial intensity profile and corresponding diffrac- tion patterns with false colors under each reaction are shown in Figure 2b,d, respectively. Instead of the three step react